Microstructure and mechanical behavior of metastable beta type titanium alloys
type: CreativeWork
description: Current biomaterials such as stainless steel, Co-Cr alloys, commercially pure titanium and Ti-6Al- 4V either possess poor mechanical compatibility and/or produce toxic effects in the human body after several years of usage. Consequently, there is an enormous demand for long-lasting biomaterials which provide a better combination of mechanical, corrosion and biological properties. In addition to this, alloys used in high-strength applications possess either high-strength or large plasticity. However, a high-strength alloy should possess a better blend of both strength and plasticity when used in high-strength applications. Metastable β-titanium alloys are the best suited alloys for biomedical and high-strength applications because they demonstrate a wide range of superior mechanical, corrosion and biological properties. In this PhD study, the Ti-27Nb-7Fe-xCr (x = 0, 2, 4, 6, 8 wt%) alloys using inexpensive elements (Fe, Mn, Cr etc.) have been designed to check their suitability for biomedical applications, whereas the Ti-33Zr-xFe-yCr (x = 3, 5, 7 and y = 2, 4 wt%), Ti-35Zr-5Fe-xMn (x = 0, 2, 4, 6, 8 wt%) and Ti-xZr-7Fe-ySn (x = 25, 30, 35 and y = 2, 4 wt%) alloys have been designed to check their suitability for high-strength applications. Later, all the investigated alloys have been cast using a cold crucible levitation melting technique. In the Ti-27Nb-7Fe-xCr alloys, only 2 wt% quantity of Cr is enough to retain a single β phase. Young’s moduli of the Ti-27Nb-7Fe-xCr alloys decrease from 116 GPa (in Ti-27Nb-7Fe) to 72 GPa (in Ti-27Nb-7Fe-8Cr) as the β stability improves. The Ti-33Zr-xFe-yCr alloys, except Ti- 33Zr-3Fe-2Cr alloy, demonstrate a C15 type Laves phase and a dominating β phase. Moreover, the Ti-35Zr-5Fe-xMn and Ti-xZr-7Fe-ySn alloys show C14 type Laves and β phases. It is quite interesting to investigate the deformation and strength characteristics of hexagonal close-packed C14 and face-centered cubic C15 type Laves phases in the soft β matrix. Therefor…
abstract: Current biomaterials such as stainless steel, Co-Cr alloys, commercially pure titanium and Ti-6Al- 4V either possess poor mechanical compatibility and/or produce toxic effects in the human body after several years of usage. Consequently, there is an enormous demand for long-lasting biomaterials which provide a better combination of mechanical, corrosion and biological properties. In addition to this, alloys used in high-strength applications possess either high-strength or large plasticity. However, a high-strength alloy should possess a better blend of both strength and plasticity when used in high-strength applications. Metastable β-titanium alloys are the best suited alloys for biomedical and high-strength applications because they demonstrate a wide range of superior mechanical, corrosion and biological properties. In this PhD study, the Ti-27Nb-7Fe-xCr (x = 0, 2, 4, 6, 8 wt%) alloys using inexpensive elements (Fe, Mn, Cr etc.) have been designed to check their suitability for biomedical applications, whereas the Ti-33Zr-xFe-yCr (x = 3, 5, 7 and y = 2, 4 wt%), Ti-35Zr-5Fe-xMn (x = 0, 2, 4, 6, 8 wt%) and Ti-xZr-7Fe-ySn (x = 25, 30, 35 and y = 2, 4 wt%) alloys have been designed to check their suitability for high-strength applications. Later, all the investigated alloys have been cast using a cold crucible levitation melting technique. In the Ti-27Nb-7Fe-xCr alloys, only 2 wt% quantity of Cr is enough to retain a single β phase. Young’s moduli of the Ti-27Nb-7Fe-xCr alloys decrease from 116 GPa (in Ti-27Nb-7Fe) to 72 GPa (in Ti-27Nb-7Fe-8Cr) as the β stability improves. The Ti-33Zr-xFe-yCr alloys, except Ti- 33Zr-3Fe-2Cr alloy, demonstrate a C15 type Laves phase and a dominating β phase. Moreover, the Ti-35Zr-5Fe-xMn and Ti-xZr-7Fe-ySn alloys show C14 type Laves and β phases. It is quite interesting to investigate the deformation and strength characteristics of hexagonal close-packed C14 and face-centered cubic C15 type Laves phases in the soft β matrix. Therefor…
author: Rabadia, Chirag Dhirajlal
keywords: Titanium alloys, Mechanical properties, Microstructure, Deformation, Fracture analysis, Engineering, Materials Science and Engineering, Mechanical Engineering
date published: 2020-01-01T08:00:00Z
date modified: 2026-07-27T19:21:17Z
provider: Edith Cowan University
publisher: Networked Digital Library of Theses and Dissertations
type: WebPage
source organization: Edith Cowan University, Research Online, Perth, Western Australia